#------------------------------------------------------------------------------
#$Date: 2023-10-07 02:57:14 +0300 (Sat, 07 Oct 2023) $
#$Revision: 286839 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/31/22/2312252.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2312252
loop_
_publ_author_name
'Shahed, H.'
'Sharma, N.'
'Angst, M.'
'Voigt, J.'
'Perßon, J'
'Prakash, P.'
'Törnroos, K W'
'Chernyshov, D.'
'Gildenast, H.'
'Ohl, M.'
'Saffarini, G.'
'Grzechnik, A.'
'Friese, K.'
_publ_section_title
;
 Structural insight into the cooperativity of spin crossover compounds.
;
_journal_issue                   'Pt 5'
_journal_name_full
'Acta crystallographica Section B, Structural science, crystal engineering and materials'
_journal_page_first              354
_journal_page_last               367
_journal_paper_doi               10.1107/S2052520623005814
_journal_volume                  79
_journal_year                    2023
_chemical_formula_sum            'C10.86 H8 Fe0.29 N1.71 S0.57'
_chemical_formula_weight         196.75
_space_group_crystal_system      orthorhombic
_space_group_IT_number           56
_space_group_name_Hall           '-P 2ab 2ac'
_space_group_name_H-M_alt        'P c c n'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2019/2
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            14
_cell_length_a                   12.9579(6)
_cell_length_b                   15.2284(7)
_cell_length_c                   17.5993(7)
_cell_measurement_reflns_used    2640
_cell_measurement_temperature    310(2)
_cell_measurement_theta_max      21.06
_cell_measurement_theta_min      1.889
_cell_volume                     3472.8(3)
_computing_structure_refinement  'SHELXL-2019/2 (Sheldrick, 2019)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.984
_diffrn_measured_fraction_theta_max 0.828
_diffrn_measurement_device_type  '4-circle diffractometer'
_diffrn_radiation_type           Synchrotron
_diffrn_radiation_wavelength     0.65524
_diffrn_reflns_av_R_equivalents  0.0974
_diffrn_reflns_av_unetI/netI     0.0728
_diffrn_reflns_Laue_measured_fraction_full 0.984
_diffrn_reflns_Laue_measured_fraction_max 0.828
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            36566
_diffrn_reflns_point_group_measured_fraction_full 0.984
_diffrn_reflns_point_group_measured_fraction_max 0.828
_diffrn_reflns_theta_full        23.150
_diffrn_reflns_theta_max         32.951
_diffrn_reflns_theta_min         1.902
_exptl_absorpt_coefficient_mu    0.433
_exptl_crystal_density_diffrn    1.317
_exptl_crystal_description       irregular
_exptl_crystal_F_000             1424
_refine_diff_density_max         0.144
_refine_diff_density_min         -0.191
_refine_diff_density_rms         0.035
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.132
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     213
_refine_ls_number_reflns         6901
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.132
_refine_ls_R_factor_all          0.2386
_refine_ls_R_factor_gt           0.1022
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0364P)²+1.2189P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1521
_refine_ls_wR_factor_ref         0.1947
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2684
_reflns_number_total             6901
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            Bia_Portho_310K.cif
_cod_data_source_block           Bia_dw4400_310K
_cod_depositor_comments
'Adding full bibliography for 2312165--2312274.cif.'
_cod_database_code               2312252
_shelx_shelxl_version_number     2019/2
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y+1/2, z'
'-x, y+1/2, -z+1/2'
'x+1/2, -y, -z+1/2'
'-x, -y, -z'
'x-1/2, y-1/2, -z'
'x, -y-1/2, z-1/2'
'-x-1/2, y, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Fe01 Fe 0.750000 0.750000 0.57587(4) 0.0720(2) Uani 1 2 d S T P . .
S002 S 0.90848(11) 0.55785(10) 0.39546(6) 0.1245(5) Uani 1 1 d . . . . .
N003 N 0.7444(2) 0.84321(18) 0.67438(15) 0.0746(7) Uani 1 1 d . . . . .
N004 N 0.8008(3) 0.6616(2) 0.49627(16) 0.0928(9) Uani 1 1 d . . . . .
N005 N 0.9099(2) 0.7962(2) 0.59376(16) 0.0789(8) Uani 1 1 d . . . . .
C006 C 0.6560(3) 0.8604(2) 0.72034(19) 0.0738(9) Uani 1 1 d . . . . .
C007 C 0.5643(3) 0.8824(2) 0.68510(19) 0.0787(9) Uani 1 1 d . . . . .
H007 H 0.561909 0.889470 0.632637 0.094 Uiso 1 1 calc R U . . .
C008 C 0.9246(3) 0.8471(3) 0.6548(2) 0.0831(10) Uani 1 1 d . . . . .
C009 C 0.8322(3) 0.8703(2) 0.6968(2) 0.0847(10) Uani 1 1 d . . . . .
H009 H 0.837101 0.905003 0.740152 0.102 Uiso 1 1 calc R U . . .
C00A C 0.6586(3) 0.8498(2) 0.7984(2) 0.0859(11) Uani 1 1 d . . . . .
H00A H 0.719839 0.834375 0.822413 0.103 Uiso 1 1 calc R U . . .
C00B C 0.4777(3) 0.8837(2) 0.8060(2) 0.0828(10) Uani 1 1 d . . . . .
C00C C 0.4764(3) 0.8938(2) 0.7280(2) 0.0844(10) Uani 1 1 d . . . . .
H00C H 0.414917 0.908544 0.703906 0.101 Uiso 1 1 calc R U . . .
C00D C 0.8458(3) 0.6192(2) 0.45406(19) 0.0783(10) Uani 1 1 d . . . . .
C00E C 0.5703(3) 0.8622(3) 0.8402(2) 0.0924(11) Uani 1 1 d . . . . .
H00E H 0.572882 0.855891 0.892679 0.111 Uiso 1 1 calc R U . . .
C00F C 0.3826(3) 0.8978(3) 0.8509(2) 0.0896(11) Uani 1 1 d . . . . .
C00G C 0.9930(3) 0.7736(3) 0.5528(2) 0.0934(11) Uani 1 1 d . . . . .
H00G H 0.984287 0.738411 0.510135 0.112 Uiso 1 1 calc R U . . .
C00H C 0.3846(4) 0.9418(3) 0.9195(2) 0.1023(13) Uani 1 1 d . . . . .
H00H H 0.447314 0.962223 0.938225 0.123 Uiso 1 1 calc R U . . .
C00I C 1.0204(4) 0.8766(3) 0.6768(3) 0.1094(14) Uani 1 1 d . . . . .
H00I H 1.027993 0.912182 0.719385 0.131 Uiso 1 1 calc R U . . .
C00J C 0.2888(4) 0.8678(3) 0.8257(3) 0.1204(15) Uani 1 1 d . . . . .
H00J H 0.285068 0.837347 0.780001 0.144 Uiso 1 1 calc R U . . .
C00K C 0.1988(4) 0.8825(4) 0.8676(3) 0.1368(18) Uani 1 1 d . . . . .
H00K H 0.135749 0.861915 0.849647 0.164 Uiso 1 1 calc R U . . .
C00L C 1.1045(4) 0.8523(4) 0.6344(3) 0.1281(17) Uani 1 1 d . . . . .
H00L H 1.170300 0.870802 0.648242 0.154 Uiso 1 1 calc R U . . .
C00M C 0.2951(5) 0.9563(3) 0.9612(3) 0.1215(16) Uani 1 1 d . . . . .
H00M H 0.298010 0.986269 1.007233 0.146 Uiso 1 1 calc R U . . .
C00N C 0.2034(5) 0.9264(4) 0.9341(3) 0.1302(18) Uani 1 1 d . . . . .
H00N H 0.143286 0.936333 0.961682 0.156 Uiso 1 1 calc R U . . .
C00O C 1.0911(4) 0.8011(4) 0.5721(3) 0.1159(15) Uani 1 1 d . . . . .
H00O H 1.147472 0.784672 0.542638 0.139 Uiso 1 1 calc R U . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Fe Fe 0.3265 0.6960 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0024 0.0013 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0049 0.0027 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1051 0.1002 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N004 Fe01 N004 93.83(18) . 2_665 ?
N004 Fe01 N005 90.30(13) . . ?
N004 Fe01 N005 100.92(12) 2_665 . ?
N004 Fe01 N005 100.92(12) . 2_665 ?
N004 Fe01 N005 90.30(13) 2_665 2_665 ?
N005 Fe01 N005 163.62(15) . 2_665 ?
N004 Fe01 N003 162.56(12) . . ?
N004 Fe01 N003 95.88(11) 2_665 . ?
N005 Fe01 N003 73.67(11) . . ?
N005 Fe01 N003 93.49(11) 2_665 . ?
N004 Fe01 N003 95.88(11) . 2_665 ?
N004 Fe01 N003 162.56(12) 2_665 2_665 ?
N005 Fe01 N003 93.49(11) . 2_665 ?
N005 Fe01 N003 73.67(11) 2_665 2_665 ?
N003 Fe01 N003 78.69(14) . 2_665 ?
C009 N003 C006 118.8(3) . . ?
C009 N003 Fe01 114.6(2) . . ?
C006 N003 Fe01 125.5(2) . . ?
C00D N004 Fe01 167.9(3) . . ?
C008 N005 C00G 117.8(3) . . ?
C008 N005 Fe01 115.6(2) . . ?
C00G N005 Fe01 126.5(3) . . ?
C007 C006 C00A 119.6(3) . . ?
C007 C006 N003 118.7(3) . . ?
C00A C006 N003 121.5(3) . . ?
C00C C007 C006 119.7(3) . . ?
N005 C008 C00I 122.9(4) . . ?
N005 C008 C009 115.6(3) . . ?
C00I C008 C009 121.5(4) . . ?
N003 C009 C008 120.0(3) . . ?
C00E C00A C006 119.7(3) . . ?
C00E C00B C00C 118.0(4) . . ?
C00E C00B C00F 121.7(3) . . ?
C00C C00B C00F 120.3(4) . . ?
C007 C00C C00B 121.4(3) . . ?
N004 C00D S002 179.0(4) . . ?
C00A C00E C00B 121.5(3) . . ?
C00J C00F C00H 117.4(4) . . ?
C00J C00F C00B 121.2(4) . . ?
C00H C00F C00B 121.4(4) . . ?
N005 C00G C00O 122.0(4) . . ?
C00F C00H C00M 121.5(5) . . ?
C00L C00I C008 118.4(5) . . ?
C00F C00J C00K 121.1(5) . . ?
C00N C00K C00J 120.0(6) . . ?
C00O C00L C00I 119.5(5) . . ?
C00N C00M C00H 119.4(5) . . ?
C00K C00N C00M 120.6(5) . . ?
C00L C00O C00G 119.4(5) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Fe01 N004 2.051(3) . ?
Fe01 N004 2.051(3) 2_665 ?
Fe01 N005 2.211(3) . ?
Fe01 N005 2.211(3) 2_665 ?
Fe01 N003 2.242(3) . ?
Fe01 N003 2.242(3) 2_665 ?
S002 C00D 1.611(4) . ?
N003 C009 1.273(4) . ?
N003 C006 1.426(4) . ?
N004 C00D 1.144(4) . ?
N005 C008 1.339(4) . ?
N005 C00G 1.340(4) . ?
C006 C007 1.382(4) . ?
C006 C00A 1.383(4) . ?
C007 C00C 1.377(5) . ?
C008 C00I 1.376(5) . ?
C008 C009 1.451(5) . ?
C00A C00E 1.373(5) . ?
C00B C00E 1.381(5) . ?
C00B C00C 1.382(5) . ?
C00B C00F 1.479(5) . ?
C00F C00J 1.372(6) . ?
C00F C00H 1.382(5) . ?
C00G C00O 1.381(6) . ?
C00H C00M 1.390(6) . ?
C00I C00L 1.372(6) . ?
C00J C00K 1.398(7) . ?
C00K C00N 1.350(7) . ?
C00L C00O 1.356(7) . ?
C00M C00N 1.359(7) . ?
